```Supplementary Information
Choice of the alignment between the (Ga,Mn)As layer and the piezoelectric actuator
The choice of aligning the (Ga,Mn)As [1-10] direction along the poling direction of
the piezoelectric actuator for both samples measured was made due to the fact that larger
voltages can be applied to these piezoelectric actuators with positive polarity rather than
negative polarity (too large negative voltages result in depolarisation of the actuators).
Details of this aspect can be found in the manufacturer’s (Piezomechanik) technical
specifications. Given that in our devices positive voltages result in a rotation of the magnetic
easy axis away from the intrinsic [1-10] direction, the choice of alignment we made allowed
to obtain a larger rotation of the easy axis. In fact, if we had aligned the (Ga,Mn)As [110]
direction along the actuator poling direction, we would have had to use negative voltages to
rotate the easy axis away from the [1-10] direction, and this would have resulted in a
smaller rotation.
Derivation of the dependence of the amplitude of the AMR on the magnetic field
In a ferromagnet for temperatures close to TC the polarization induced by a magnetic
field B on the magnetic moments is non negligible and results in a dependence of the
saturation magnetization MS at that temperature on B [1]. Since the amplitude R of the
AMR is influenced by the value of MS, the dependence of MS on B determines a dependence
of R on B [2].
Within an approximation of ~ 10 % the transverse AMR is given by Rxy = Rsin(2)
[3], where  is the angle between the direction of M and the current direction [1-10] in the
1
Hall bar. Fig. S1(a) shows Rxy as a function of B when B is applied in the plane of the Hall bar
at the angles  = -45° and  = +45° to the [1-10] direction. For saturating B (for which  = ),
these angles are those at which Rxy is respectively maximum and minimum (R < 0), as
displayed by the inset in Fig. S1(a). Therefore, for saturating B, R(B) can be simply derived
by averaging the upper and lower branches for each loop in Fig. S1(a), taking their
difference and dividing it by 2. R(B) thus obtained is shown for |B| > 45 mT by the symbols
in Fig. S1(b), alongside with the curve R(B) = R0 + a|B| + b|B|1/3 used to fit to it, with R0
= -0.575, a = -0.029 and b = -0.312.
This expression of R(B), which fits very well to the experimental data, is the one
used for the analysis of the magneto-transport data described in the paper.
1.0
(a)
(b)
Data
Fit
-0.6
o
1
 = -45
o
 = +45
R ()
B = 60 mT
Rxy ()
Rxy ()
0.5
0.0
0
-1
-90
-0.5
-45
0
 (deg)
45
90
-1.0
-600
-300
0
B (mT)
300
600
-0.7
-0.8
-0.9
-600
-300
0
300
600
B (mT)
Fig. S1 (a) Transverse resistance Rxy measured at T = 150 K and VP = 0 V as a function of the
external magnetic field B applied at  = -45° and  = +45°. B is swept from +600 mT to -600
mT and back to +600 mT. The inset shows Rxy measured at T = 150 K as a function of , the
angle of the applied B, for B = 60 mT. (b) Amplitude R of the AMR at T = 150 K as a function
of B. The symbols are the experimental data obtained from [ xy( = +45°) -  xy( = -45°)]/2
for |B| > 45 mT ( xy is used to indicate the average between the upper and lower branches),
while the solid line is the result of their fitting with R(B) = R0 + a|B| + b|B|1/3.
2
References
[1] S. Blundell, Magnetism in Condensed Matter (Oxford University Press, Oxford, 2001).
[2] J. A. Haigh, A. W. Rushforth, C. S. King, K. W. Edmonds, R. P. Campion, C. T. Foxon, and B.
L. Gallagher, Appl. Phys. Lett. 95, 232102 (2009).
[3] A. W. Rushforth, K. Výborný, C. S. King, K. W. Edmonds, R. P. Campion, C. T. Foxon, J.
Wunderlich, A. C. Irvine, P. Vašek, V. Novák, K. Olejník, Jairo Sinova, T. Jungwirth, and B. L.
Gallagher, Phys. Rev. Lett. 99, 147207 (2007).
3
```